M2 high speed tool steel is tungsten-molybdenum high-speed steel with a well-balanced carbon composition and high toughness. It is also called JIS SKH51 and DIN 1.3343 steel. It is easy to overheat, control the quenching heating temperature is necessary and the heat treatment protection requirements are strict. It is used widely to make cutting tools because of its great hardness and wear resistance. It has replaced T1 high speed steel in most applications, become the first choice of customer due to its great performance and extremely high-performance price ratio. M2 steel round bar sheet plate properties and heat treat as below.
1.3343 Steel Characteristics
- Hardness(Factory original status): ≤255HB
- Hardening temperature: 1220℃-1240℃
- Hardness(After heat treatment): ≤63HRC
- It is a great choice at cutting applications due to its great wear resistance and toughness.
- Carbide uniformly distributed and high toughness.
- It can be used to make milling cutters, reamers, broaches, gear cutters and other industry tools.
1.3343 Steel Application
The application is decided by M2 steel chemical composition and properties. It has high hardness, red hardness. Good thermoplasticity and excellent toughness. It is used to make tools that require has good wear resistance and toughness which can sustain large impact forces. Such as pinion cutters, planers, milling cutters, turning tools, drill bits and etc.
M2 Steel Mechanical Properties
|Hardness, Rockwell C(tempered at 1150°F, quenched at 2200°F)||62||62|
|Hardness, Rockwell C(as hardened, quenched at 2200°F)||65||65|
|Compressive yield strength(when tempered at 300°F)||3250 MPa||471000 psi|
|Izod impact unnotched(when tempered at 300°F)||67 J||49.4 ft-lb|
|Abrasion(loss in mm3, as-hardened; ASTM G65)||25.8||25.8|
|Abrasion(loss in mm3, tempered at 1275°F; ASTM G65)||77.7||77.7|
|Elastic modulus||190-210 GPa||27557-30458 ksi|
1.3343 Steel Physical Properties
|Density||8.16 g/cm³||0.294 lb/in³|
M2 Steel Grade Equivalent Chart
|Standard||ASTM A600-92a||EN ISO 4957-1999||JIS G4403-2006||ISO 4957-1999|
|Grades||M2(Standard C)||HS 6-5-2||SKH51||HS 6-5-2|
M2 Steel Chemical Composition
|ASTM A600-92a||0.78-0.88||0.15-0.40||Max 0.03||Max 0.03||0.20-0.45||3.75-4.50||1.75-2.20||5.50-6.75||4.50-5.50|
|EN ISO 4957-1999||0.80-0.88||≤0.40||≤0.030||≤0.030||≤0.45||3.80-4.50||1.70-2.10||5.90-6.70||4.70-5.20|
|JIS G4403-2006||0.80-0.88||Max 0.40||Max 0.030||Max 0.030||Max 0.45||3.80-4.50||1.70-2.10||5.90-6.70||4.70-5.20|
M2 Steel Round Bar Sheet Plate Heat Treatment
The shaping of M2 tool steels may be executed using grinding strategies. But, which has bad grinding capability. So they’re called as “medium” machinability tool steel under annealed conditions. The machinability of these steels is only 50% of that of the easily machinable W group or water hardening tool steels.
Heat to 1600° F, soak thoroughly at heat. Furnace cool 25° F per hour to 900° F, air cool to room temperature. Approximate annealed hardness 241 Maximum Brinell.
Stress Relief of Unhardened Material: Heat slowly to 1200 to 1250° F. Soak for two hours per inch of thickness at heat. Slow cool(furnace cool if possible) to room temperature.
Heat M2 steel slowly to 1550° F, soak fully, heat to 1850° F, soak thoroughly. Soak time in the furnace varies from a few minutes to 15 minutes, depending on tool size, the heat capacity of the furnace, and the size of the charge. – Heat to 2150 to 2200° F for max. toughness and minimum distortion. – Heat to 2250 to 2275° F for max.
Double tempering is necessary, sometimes preferred three times tempering. Soak for 2 hours per inch of thickness. Air cool to room temperature between tempers. The best tempering range for hardness, strength and toughness is 1000 to 1050° F.
For full hardness, need to oil quench to 150-200° F. Air quenches to 150° F. When quenching in hot salt maintains the quench just above the Ms temperature. After equalizing withdraw parts from the hot salt and air cooled to 150° F.
M2 Steel Heat Treatment
M2 high speed steel is preheated prior to hardening at 2610 ° C(4730 ° F). Then heated rapidly from 2610 ° C (4730 ° F) to 3960 ° C (7160 ° F). The steel is finally cooled for 3 to 5 minutes and quenched in air, salt bath or oil.
M2 Steel Quality Certificate
M2 Tool Steel Round Bar Sheet Plate Supply
Specification: Dia 12-220mm; Length: Can be customized
Surface: Black Surface/Bright Surface /Grinded/Peeled/Turned
Specification: thickness: 3-200mm; width: Can be customized; length: Can be customized
Surface: Black Surface/Bright Surface /Grinded/Peeled/Turned
We have our own cutting and processing equipment. Specifications can be cut and customized according to your requirements.
We are a professional special steel stockist and supplier with a high-quality stand for many years. As a professional M2 steel supplier, please contacts us for any request of AISI M2/DIN 1.3343 steels materials. Songshun Steel always with you.
AISI 6150 steel is an alloy spring steel. It has great mechanical properties......
AISI 52100 steel is the representative of high carbon chromium bearing steel type.
4130 alloy steel has high strength and toughness and the hardenability is high.
It has great mechanical property and processability. And it is great choice for the production of the.....
AISI 5140 steel also can be called JIS Scr440 and DIN 1.7035 steel. It is one of the alloy steel.
AISI O2 steel is the better type compare with the O1 tool steel. Its content of carbon, chromium and tungsten has been raised.
M35 steel is high speed tool steel. After the heat treatment, its hardness, red hardness and wear resistance can be.....
12L14 is a free cutting structural steel. And it is easy to be machined.
1045 carbon steel has a tensile strength is 570-700 MPa and Brinell hardness ranging between 170 and 210.
8620 steel is alloy steel and has good strength and toughness properties. This alloy steel is flexible during....
4340 steel has great machinability, heat treatment stability and impact toughness.
4140 steel is an alloy structural steel with high strength, hardenability, good toughness....
T1 HSS tool steel is the most widely used tungsten type of high speed steel. Its properties are great, has good abrasion, toughness and hardness.
M42 high-speed steel is a cobalt-molybdenum tools steel. The addition of 8% cobalt means that M42 has superior red-hardness when....
AISI M2 high-speed steel has largely replaced T1 in most applications due to its superior properties and advantageous pricing. It is a medium....
According to the AISI classification system, chromium hot-work tool steels are designated as group H steels.
The hardness of A2 steel after heat treatment is higher than SKD11 steel. Its hardness could reach 60-62HRC after....